 Nano Express
 Open Access
 Published:
Doping dependence of lowenergy quasiparticle excitations in superconducting Bi2212
Nanoscale Research Letters volume 8, Article number: 515 (2013)
Abstract
The dopingdependent evolution of the dwave superconducting state is studied from the perspective of the angleresolved photoemission spectra of a highT_{c} cuprate, Bi_{2}Sr_{2}CaCu_{2} O_{8+δ} (Bi2212). The anisotropic evolution of the energy gap for Bogoliubov quasiparticles is parametrized by critical temperature and superfluid density. The renormalization of nodal quasiparticles is evaluated in terms of mass enhancement spectra. These quantities shed light on the strong coupling nature of electron pairing and the impact of forward elastic or inelastic scatterings. We suggest that the quasiparticle excitations in the superconducting cuprates are profoundly affected by dopingdependent screening.
Background
Electronic excitations dressed by the interaction with the medium are called quasiparticles. They serve as a direct probe of the anisotropic order parameter of a superconducting phase and also as a clue to the electronpairing glue responsible for the superconductivity. In fact, the major unresolved issues on the mechanism of highT_{c} superconductivity depend on the lowenergy quasiparticle excitations. The superconducting order parameter, which is typified by the particlehole mixing and gives rise to Bogoliubov quasiparticles (BQPs), manifests itself as an energy gap in quasiparticle excitation spectra. In cuprate superconductors, however, the energy gap increases against the decrease in critical temperature T_{c} with underdoping and is open even at some temperatures above T_{c}[1–3]. In the direction where the dwave order parameter disappears, renormalization features have been extracted quantitatively from the gapless continuous dispersion of nodal quasiparticles (NQPs), suggesting strong coupling with some collective modes[4]. Nevertheless, the origins of these features remain controversial[4, 5].
In this paper, we address the doping dependence of BQP and NQP of a highT_{c} cuprate superconductor, Bi_{2}Sr_{2}CaCu_{2}O_{8+δ} (Bi2212), on the basis of our recent angleresolved photoemission (ARPES) data[6–8]. The use of lowenergy synchrotron radiation brought about improvement in energy and momentum resolution and allowed us to optimize the excitation photon energy. After a brief description of BQP and NQP spectral functions, we survey the superconducting gap anisotropy on BQPs and the renormalization features in NQPs. In light of them, we discuss possible effects of dopingdependent electronic screening on the BQP, NQP, and highT_{c} superconductivity.
Methods
Highquality single crystals of Bi2212 were prepared by a travelingsolvent floatingzone method, and hole concentration was regulated by a postannealing procedure. In this paper, the samples are labeled by the T_{c} value in kelvin, together with the dopinglevel prefix, i.e. underdoped (UD), optimally doped (OP), or overdoped (OD). ARPES experiments were performed at HiSOR BL9A in Hiroshima Synchrotron Radiation Center. The ARPES data presented here were taken with excitationphoton energies of h ν = 8.5 and 8.1 eV for the BQP and NQP studies, respectively, and at a low temperature of T = 9  10 K in the superconducting state. Further details of the experiments have been described elsewhere[7–9].
The relation between a bare electron and a renormalized quasiparticle is described in terms of selfenergy Σ_{ k }(t), which can be regarded as a factor of feedback on the wave function from past to present through the surrounding medium. Incorporating a feedback term into the Schrödinger equation, we obtain
where ψ_{ k }(t) and{\omega}_{\mathbf{k}}^{0} denote a wave function and a bareelectron energy, respectively. It is obvious from Equation 1 that the selfenergy is a linear response function. Therefore, its frequency representation, Σ_{ k }(ω), obeys the KramersKronig relation. As the solution of Equation 1, we obtain the form of dressed Green’s function,
The spectral function given by A_{ k }(ω) =  Im G_{ k }(ω)/π is directly observed by ARPES experiments. The extensive treatments of the ARPES data in terms of Green’s function are given elsewhere[10].
Results
Superconducting gap anisotropy
In the superconducting state, the condensate of electron pairs allows the particlelike and holelike excitations to turn into each other. Hence, the wave function of a holelike excitation also comes back by way of the particlelike excitation. Such a feedback has a signreversed eigenenergy,{\omega}_{\mathbf{k}}^{0}, and is expressed by{\mathrm{\Sigma}}_{\mathbf{k}}(t)=i\mathrm{\Theta}(t){\mathrm{\Delta}}_{\mathbf{k}}^{2}{e}^{i{\omega}_{\mathbf{k}}^{0}t}{e}^{{\gamma}_{\mathbf{k}}t}i{\mathrm{\Gamma}}_{\mathbf{k}}\delta (t), where Θ(t), Δ_{ k }, γ_{ k } and Γ_{ k } denote the step function, the particlehole offdiagonal element, and the scattering rates of the intermediate and bareparticle states, respectively. The Fourier transform of Σ_{ k }(t) gives the frequency representation of the selfenergy of the BQPs,
Figure1 shows the ARPES spectra of BQPs for underdoped and overdoped Bi2212 samples with T_{c} = 66 and 80 K (UD66 and OD80, respectively)[8]. As shown in Figure1b,c, an energy distribution curve was extracted from the minimum gap locus for each offnode angle θ and symmetrized with respect to the Fermi energy ω = 0. These spectra were well fitted with a phenomenological function,
except for a featureless background. Equation 4 is deduced from Equation 3 and{\omega}_{\mathbf{k}}^{0}=0, neglecting γ_{ k } after Norman et al.[11]. Figure1b,c exemplifies that the superconducting gap energy Δ at each θ is definitely determined by sharp spectral peaks. In Figure1d,e, the obtained gap energies (small yellow circles) are plotted over the image of spectral intensity as a function of sin 2θ, so that the deviation from a dwave gap is readily seen with reference to a straight line. While the superconducting gap of the overdoped sample almost follows the dwave line, that of the underdoped sample is deeply curved against sin 2θ. Furthermore, Figure1d indicates that the deviation from the dwave gap penetrates into the close vicinity of the node and that it is difficult to define the pure dwave region near the node. Therefore, the nextorder harmonic term, sin 6θ, has been introduced, so that the smooth experimental gap profile is properly parametrized[12–14]. The nextorder highharmonic function is also expressed as Δ(θ) = Δ_{N} sin 2θ + (Δ^{∗}Δ_{N})(3 sin 2θ sin 6θ)/4, where the antinodal and nodal gap energies are defined as Δ^{∗} = Δ(θ)_{θ=45°} and{\mathrm{\Delta}}_{\mathrm{N}}={\left(\right)close="">\frac{1}{2}(d\mathrm{\Delta}/d\theta )}_{}\n \n \theta \n =\n 0\n \n, respectively, so that Δ_{N}/Δ^{∗} = 1 is satisfied for a pure dwave gap.
The doping dependences of the superconducting gap parameters are summarized in Figure2. One can see from Figure2a that as hole concentration decreases with underdoping, the nodal gap energy 2Δ_{N} closely follows the downward curve of 8.5k_{B}T_{c} in contrast to the monotonic increase in the antinodal gap energy 2Δ^{∗}. It seems reasonable that T_{c} primarily depends on Δ_{N} rather than Δ^{∗} for the underdoped Bi2212, because it follows from 2Δ^{∗} ≫ 4k_{B}T_{c} that the thermal quasiparticle excitations concentrate in the vicinity of the node and hardly occur around the antinode. The relevance of the nodal excitations has also been suggested by various experiments[15–19]. Then, the problem with T_{c} is that the nodal gap Δ_{N} is suppressed relative to the antinodal gap Δ^{∗}. This behavior can be associated with low superfluid density ρ_{s}[20]. Figure2b,c shows that the doping dependence of the nodaltoantinodal gap ratio Δ_{N}/Δ^{∗} is quite similar to that of the squareroot superfluid density\sqrt{{\rho}_{\mathrm{s}}}[8, 21, 22]. The normalized gap plot in Figure2d indicates that what occurs with underdoping is analogous to the nodal gap suppression observed with increasing temperature[17] in terms of the decrease in ρ_{s}. It is notable that the squareroot dependence on ρ_{s} is a typical behavior of the order parameter as expected from the GinzburgLandau theory[23]. These findings can be written down in a simple relational formula,
where{\rho}_{\mathrm{s}}^{0}\simeq 31\mu {\mathrm{m}}^{2}, for a wide holeconcentration range of Bi2212.
As presented in Figure2e, the correlation between the nodal and antinodal gaps provides a perspective of crossover for our empirical formula (Equation 5). It is deduced from the conventional BardeenCooperSchrieffer (BCS) theory that 2Δ/k_{B}T_{c} = 4.3 in the weak coupling limit for the dwave superconducting gap[23]. However, the critical temperature T_{c} is often lower than that expected from the weak coupling constant and a given Δ as an effect of strong coupling. Thus, the gapto T_{c} ratio is widely regarded as an indicator for the coupling strength of electron pairing and adopted for the coordinate axes in Figure2e. As hole concentration decreases from overdoped to underdoped Bi2212, the experimental data point moves apart from the weak coupling point toward the strong coupling side, and a crossover occurs at 8.5, which is about twice the weak coupling constant. It appears that the evolution of Δ_{N} is confined by two lines as Δ_{N} ≤ 0.87Δ^{∗} and 2Δ_{N} ≤ 8.5k_{B}T_{c}. As illustrated in the insets of Figure2e, the strong coupling allows the electrons to remain paired with incoherent excitations. As a result, the superconducting order parameter is reduced with respect to the pairing energy. Indeed, it has been shown that the reduction factor due to the incoherent pair excitations has a simple theoretical expression\sqrt{{\rho}_{\mathrm{s}}/{\rho}_{\mathrm{s}}^{\text{BCS}}} and that the nodal and antinodal spectra are peaked at the order parameter and at the pairing energy, respectively, taking into account a realistic lifetime effect[24, 25]. Therefore, the latter part of Equation 5 is consistent with the strong coupling scenario, and furthermore, the two distinct lines in Figure2e are naturally interpreted as the energies of the condensation and formation of the electron pairs.
Renormalization features in dispersion
In the nodal direction where the order parameter disappears, one can investigate the fine renormalization features in dispersion. They reflect the intermediatestate energy in coupling between an electron and other excitations, and thus provide important clues to the pairing interaction. As for the electronboson coupling, the intermediate state consists of a dressed electronic excitation and an additional bosonic excitation (Figure3a). Averaging the momentum dependence for simplicity, the energy distribution of the intermediate state is expressed by A(ω  Ω) Θ(ω  Ω)+A(ω + Ω) Θ(ω  Ω) for a given boson energy Ω and for zero temperature, owing to the Pauli exclusion principle. Therefore, taking into account the effective energy distribution of the coupled boson, α^{2}F(Ω), the selfenergy is written down as follows:
where 0^{+} denotes a positive infinitesimal.
In ARPES spectra, the real and imaginary parts of selfenergy manifest themselves as the shift and width of spectral peak, respectively. Specifically, provided that the momentum dependence of Σ_{ k }(ω) along the cut is negligible, and introducing bare electron velocity v_{0} by{\omega}_{k}^{0}={v}_{0}k, it follows from Equation 2 that the momentum distribution curve for a given quasiparticle energy ω is peaked at k(ω) = [ωReΣ(ω)]/v_{0} and has a natural half width of Δk(ω) =  ImΣ(ω)/v_{0}.
We argue that the mass enhancement function defined as the energy derivative of the selfenergy, λ(ω) ≡ (d/d ω)Σ(ω), is useful for the analysis of NQP[7, 26]. The real and imaginary parts of λ(ω) are directly obtained from the ARPES data as the inverse of group velocity, v_{g}(ω), and as the differential scattering rate, respectively.
We note that Imλ(ω) represents the energy distribution of the impact of coupling with other excitations and can be taken as a kind of coupling spectrum. However, it should be emphasized that Imλ(ω) is expressed as a function of quasiparticle energy ω, whereas the widely used Eliashberg coupling function α^{2}F(Ω) is expressed as a function of boson energy Ω. For example, a simulation of λ(ω) using Equations 7 to 9 is presented in Figure3b,c, where a single coupling mode is given at Ω = 40 meV. One can see that the peak of α^{2}F(ω) is reproduced by Imλ(ω), provided that A(ω) is gapless and approximated by a constant. As an energy gap of Δ opens in A(ω), the peak in Imλ(ω) is shifted from Ω into Ω + Δ. Nevertheless, irrespective of A(ω), the causality of Σ(ω) is inherited by λ(ω), so that Reλ(ω) and Imλ(ω) are mutually convertible through the KramersKronig transform (KKT). The directness and causality of λ(ω) enable us to decompose the quasiparticle effective mass without tackling the integral inversion problem in Equation 7.
Figure4 shows the ARPES spectra along the nodal cut perpendicular to the Fermi surface for the superconducting Bi2212[7]. Although the splitting due to the CuO_{2} bilayer is minimum at the nodes, it has clearly been observed by using some specific lowenergy photons[6–8]. A prominent kink in the NQP dispersion is observed at 65 meV for all the doping level, as has been reported since early years[4]. In addition to this, another small kink at 15 meV is discernible in the raw spectral image of the underdoped sample (UD66)[7, 27].
The fine renormalization features in the NQP dispersion were determined by fitting the momentum distribution curves with double Lorentzian. Figure5a,d shows the real and imaginary parts of λ(ω)/v_{0} experimentally obtained as the energy derivatives of the peak position and width, respectively. The KKT of Reλ(ω)/v_{0} in Figure5a is shown in Figure5b as Imλ(ω)/v_{0}, which is comparable with the data in Figure5d. A steplike mass enhancement in Figure5a and a peaklike coupling weight in Figure5b,d are consistently observed at 65 meV. This is a typical behavior of the mode coupling, as shown by the simulation in Figure3. It is also found that an additional feature around 15 meV is dramatically enhanced with underdoping. In order to deduce the partial coupling constant, we express the mass enhancement factor λ as the form of KKT,
Dividing the energy range of the integral in Equation 10, one can quantify the contribution from a particular energy part. We refer to the KKT integrals of Im λ(ω)/v_{0} for the lowenergy (LE; 4 < ω < 40 meV), intermediateenergy (IE; 40 < ω < 130 meV), and highenergy (HE; 130 < ω < 250 meV) parts as λ^{LE}/v_{0} (red circles), λ^{IE}/v_{0} (blue triangles), and λ^{HE}/v_{0} (green diamonds), respectively. Those obtained from the data in Figure5b,d are plotted in Figure5c,e, respectively. Also shown in Figure5c are the inverse group velocities at ω = 0 meV (black circles) and at ω = 40 meV (black triangles). Figure5c and Figure5e consistently indicate that as hole concentration decreases, the contribution of the lowenergy part rapidly increases and becomes dominant over the other parts.
Possible origins of the lowenergy kink are considered from the energy of 15 meV and the evolution with underdoping. The quasiparticles that can be involved in the intermediate states are limited within the energy range of ω ≤ 15 meV, and the irrelevance of the antinodal states is deduced from the simulation in Figure3c. Therefore, the lowenergy kink is due to the nearnodal scatterings with small momentum transfer. The candidates for bosonic forward scatterers are the lowfrequency phonons, such as the acoustic phonons and the caxis optical phonons involving heavy cations[7, 28–31]. On the other hand, it has also been argued that the elastic forward scattering by offplane impurities may give rise to the lowenergy kink for the dwave superconductors[7, 32]. In usual metal, both the potentials of the lowfrequency phonons and the static impurities are strongly screened by the rapid response of electronic excitations. Therefore, the enhancement of the lowenergy kink suggests the breakdown of electronic screening at low hole concentrations[7, 28].
The dispersion kink at 65 meV has been ascribed to an intermediate state consisting of an antinodal quasiparticle and the B_{1g} buckling phonon of Ω ∼ 35 meV[33]. However, the mass enhancement spectra in Figure5a,b,d are suggestive of the presence of multiple components in the intermediateenergy range.
Discussion
We found that both the superconducting gap anisotropy and the renormalized dispersion show the striking evolution with underdoping. These behaviors are considered to be dependent on the extent of the screening. In association with the forward elastic or inelastic scatterings, the screening breakdown would enhance the lowenergy kink. From the aspect of the impact of offplane impurities, the inadequacy of static screening would inevitably lead to the nanoscale inhomogeneities, as observed by scanning tunneling microscopy experiments[34]. The forward scatterings by the remaining potential would generate additional incoherent pair excitations, as expected from the nodal gap suppression at low temperatures[8, 25]. From the aspect of the electronphonon coupling, the inhomogeneous depletion of the electrons for screening may considerably increase the coupling strength, providing an account for the unexpectedly strong dispersion kink[35] and a candidate for the strong pairing interaction[8]. The former and latter aspects have negative and positive effects, respectively, on the superconductivity. Thus, we speculate that the doping dependence of T_{c} is eventually determined by the balance between these effects.
Conclusions
Summarizing, the evolution of a dwave highT_{c} superconducting state with hole concentration has been depicted on the basis of the highresolution ARPES spectra of the quasiparticles and discussed in relation to the screening by electronic excitations. The divergence between the nodal and antinodal gaps can be interpreted as an effect of the incoherent pair excitations inherent in the strong coupling superconductivity. The lowenergy kink, which rapidly increases with underdoping, should be caused by the forward elastic or inelastic scatterings, although it remains as an open question which scattering is more dominant. The quantitative simulation of the dopingdependent effect will be helpful for resolving this problem.
Abbreviations
 AB:

Antibonding band
 ARPES:

Angleresolved photoemission spectroscopy
 BB:

Bonding band
 BCS:

BardeenCooperSchrieffer
 Bi2212:

Bi_{2}Sr_{2}CaCu_{2} O_{8+δ}
 BQP:

Bogoliubov quasiparticle
 HE:

High energy
 IE:

Intermediate energy
 KKT:

KramersKronig transform
 LE:

Low energy
 NQP:

Nodal quasiparticle
 OD:

Overdoped
 OP:

Optimally doped
 UD:

Underdoped.
References
 1.
Miyakawa N, Guptasarma P, Zasadzinski JF, Hinks DG, Gray KE: Strong dependence of the superconducting gap on oxygen doping from tunneling measurements on Bi_{2}Sr_{2}CaCu_{2}O_{8δ}. Phys Rev Lett 1998, 80: 157–160. 10.1103/PhysRevLett.80.157
 2.
Campuzano JC, Ding H, Norman MR, Fretwell HM, Randeria M, Kaminski A, Mesot J, Takeuchi T, Sato T, Yokoya T, Takahashi T, Mochiku T, Kadowaki K, Guptasarma P, Hinks DG, Konstantinovic Z, Li ZZ, Raffy H: Electronic spectra and their relation to the ( π,π ) collective mode in high T_{ c } superconductors. Phys Rev Lett 1999, 83: 3709–3712. 10.1103/PhysRevLett.83.3709
 3.
Loeser AG, Shen ZX, Dessau DS, Marshall DS, Park CH, Fournier P, Kapitulnik A: Excitation gap in the normal state of underdoped Bi_{2}Sr_{2}CaCu_{2}O_{8+δ}. Science 1996, 273: 325–329. 10.1126/science.273.5273.325
 4.
Lanzara A, Bogdanov PV, Zhou XJ, Kellar SA, Feng DL, Lu ED, Yoshida T, Eisaki H, Fujimori A, Kishio K, Shimoyama JI, Noda T, Uchida S, Hussain Z, Shen ZX: Evidence for ubiquitous strong electronphonon coupling in hightemperature superconductors. Nature 2001, 412: 510. 10.1038/35087518
 5.
Johnson PD, Valla T, Fedorov AV, Yusof Z, Wells BO, Li Q, Moodenbaugh AR, Gu GD, Koshizuka N, Kendziora C, Jian S, Hinks DG: Doping and temperature dependence of the mass enhancement observed in the cuprate Bi_{2}Sr_{2}CaCu_{2}O_{8+δ}. Phys Rev Lett 2001, 87(17):177007.
 6.
Yamasaki T, Yamazaki K, Ino A, Arita M, Namatame H, Taniguchi M, Fujimori A, Shen ZX, Ishikado M, Uchida S: Unmasking the nodal quasiparticle dynamics in cuprate superconductors using lowenergy photoemission. Phys Rev B 2007, 75: 140513.
 7.
Anzai H, Ino A, Kamo T, Fujita T, Arita M, Namatame H, Taniguchi M, Fujimori A, Shen ZX, Ishikado M, Uchida S: Energydependent enhancement of the electroncoupling spectrum of the underdoped Bi_{2}Sr_{2}CaCu_{2}O_{8+δ} superconductor. Phys Rev Lett 2010, 105: 227002.
 8.
Anzai H, Ino A, Arita M, Namatame H, Taniguchi M, Ishikado M, Fujita K, Ishida S, Uchida S: Relation between the nodal and antinodal gap and critical temperature in superconducting Bi2212. Nat Commun 1815, 4: 2013.
 9.
Hobou H, Ishida S, Fujita K, Ishikado M, Kojima KM, Eisaki H, Uchida S: Enhancement of the superconducting critical temperature in Bi_{2}Sr_{2}CaCu_{2}O_{8+δ} by controlling disorder outside CuO_{2} planes. Phys Rev B 2009, 79: 064507.
 10.
Campuzano JC, Norman MR, Randeria M: Photoemission in the High T_{ c } Superconductors. In The Physics of Superconductors. Edited by: Bennemann KH, Ketterson JB. Berlin: Springer; 2004:167–273. [ArXiv/0209476] [ArXiv/0209476]
 11.
Norman MR, Randeria M, Ding H, Campuzano JC: Phenomenology of the lowenergy spectral function in high T_{ c } superconductors. Phys Rev B 1998, 57: 11093–11096. 10.1103/PhysRevB.57.R11093
 12.
Mesot J, Norman MR, Ding H, Randeria M, Campuzano JC, Paramekanti A, Fretwell HM, Kaminski A, Takeuchi T, Yokoya T, Sato T, Takahashi T, Mochiku T, Kadowaki K: Superconducting gap anisotropy and quasiparticle interactions: a doping dependent photoemission study. Phys Rev Lett 1999, 83(4):840. 10.1103/PhysRevLett.83.840
 13.
Angilella GGN, Sudbø A, Pucci R: Extendedwave superconductivity. Flat nodes in the gap and the lowtemperature asymptotic properties of highsuperconductors. Eur Phys J B 2000, 15(2):269–275.
 14.
Angilella GGN, Pucci R, Siringo F, Sudbø A: Sharp kspace features in the order parameter within the interlayer pairtunneling mechanism of high T_{ c } superconductivity. Phys Rev B 1999, 59: 1339–1353. 10.1103/PhysRevB.59.1339
 15.
Tacon ML, Sacuto A, Georges A, Kotliar G, Gallais Y, Colson D, Forget A: Two energy scales and two distinct quasiparticle dynamics in the superconducting state of underdoped cuprates. Nat Phys 2006, 2: 537–543. 10.1038/nphys362
 16.
Alldredge JW, Lee J, McElroy K, Wang M, Fujita K, Kohsaka Y, Taylor C, Eisaki H, Uchida S, Hirschfeld PJ, Davis JC: Evolution of the electronic excitation spectrum with strongly diminishing hole density in superconducting Bi_{2}Sr_{2}CaCu_{2}O_{8+δ}. Nat Phys 2008, 4: 319–326. 10.1038/nphys917
 17.
Lee WS, Vishik IM, Tanaka K, Lu DH, Sasagawa T, Nagaosa N, Devereaux TP, Hussain Z, Shen ZX: Abrupt onset of a second energy gap at the superconducting transition of underdoped Bi2212. Nature 2007, 450: 81–84. 10.1038/nature06219
 18.
Pushp A, Parker CV, Pasupathy AN, Gomes KK, Ono S, Wen J, Xu Z, Gu G, Yazdani A: Extending universal nodal excitations optimizes superconductivity in Bi_{2}Sr_{2}CaCu_{2}O_{8+δ}. Science 2009, 324(5935):1689–1693. 10.1126/science.1174338
 19.
Tanaka K, Lee WS, Lu DH, Fujimori A, Fujii T, Risdiana , Terasaki I, Scalapino DJ, Devereaux TP, Hussain Z, Shen ZX: Distinct Fermimomentumdependent energy gaps in deeply underdoped Bi2212. Science 2006, 314(5807):1910–1913. 10.1126/science.1133411
 20.
Emery VJ, Kivelson SA: Importance of phase fluctuations in superconductors with small superfluid density. Nature 1995, 374(6521):434–437. 10.1038/374434a0
 21.
Anukool W, Barakat S, Panagopoulos C, Cooper JR: Effect of hole doping on the London penetration depth in Bi_{2}Sr_{1.85}CaCu_{2}O_{8+δ} and Bi_{2.1}Sr_{1.9}Ca_{0.85}Y_{0.15}Cu_{2}O_{8+δ}. Phys Rev B 2009, 80: 024516.
 22.
Tallon JL, Loram JW, Cooper JR, Panagopoulos C, Bernhard C: Superfluid density in cuprate high T_{ c } superconductors: a new paradigm. Phys Rev B 2003, 68: 180501.
 23.
Schrieffer JR: Theory of Superconductivity. New York: AddisonWesley; 1964.
 24.
Chen Q, Kosztin I, Boldizsár J, Levin K: Pairing fluctuation theory of superconducting properties in underdoped to overdoped cuprates. Phys Rev Lett 1998, 81: 4708–4711. 10.1103/PhysRevLett.81.4708
 25.
Chien CC, He Y, Chen Q, Levin K: Twoenergygap preformedpair scenario for cuprate superconductors: implications for angleresolved photoemission spectroscopy. Phys Rev B 2009, 79: 214527.
 26.
Mahan GD: ManyParticle Physics. New York: Plenum; 1981.
 27.
Vishik IM, Lee WS, Schmitt F, Moritz B, Sasagawa T, Uchida S, Fujita K, Ishida S, Zhang C, Devereaux TP, Shen ZX: Dopingdependent nodal Fermi velocity of the hightemperature superconductor Bi_{2}Sr_{2}CaCu_{2}O_{8+δ} revealed using highresolution angleresolved photoemission spectroscopy. Phys Rev Lett 2010, 104: 207002.
 28.
Johnston S, Vishik IM, Lee WS, Schmitt F, Uchida S, Fujita K, Ishida S, Nagaosa N, Shen ZX, Devereaux TP: Evidence for the importance of extended Coulomb interactions and forward scattering in cuprate superconductors. Phys Rev Lett 2012, 108: 166404.
 29.
Rameau JD, Yang HB, Gu GD, Johnson PD: Coupling of lowenergy electrons in the optimally doped Bi_{2}Sr_{2}CaCu_{2}O_{8+δ} superconductor to an optical phonon mode. Phys Rev B 2009, 80: 184513.
 30.
Kovaleva NN, Boris AV, Holden T, Ulrich C, Liang B, Lin CT, Keimer B, Bernhard C, Tallon JL, Munzar D, Stoneham AM: c axis lattice dynamics in Bibased cuprate superconductors. Phys Rev B 2004, 69: 054511.
 31.
Kulić ML: Interplay of electronphonon interaction and strong correlations: the possible way to hightemperature superconductivity. Phys Rep 2000, 338: 1–264. 10.1016/S03701573(00)000089
 32.
Hong SH, Bok JM, Choi HY, Zhang W, He J, Zhou XJ: Low energy kink induced by offplane impurities in BSCCO superconductors. arXiv/1306.3731
 33.
Devereaux TP, Cuk T, Shen ZX, Nagaosa N: Anisotropic electronphonon interaction in the cuprates. Phys Rev Lett 2004, 93: 117004.
 34.
McElroy K, Lee D, Hoffman J, Lang K, Lee J, Hudson E, Eisaki H, Uchida S, Davis J: Coincidence of checkerboard charge order and antinodal state decoherence in strongly underdoped superconducting Bi_{2}Sr_{2}CaCu_{2}O_{8+δ}. Phys Rev Lett 2005, 94(19):197005.
 35.
Giustino F, Cohen ML, Louie SG: Small phonon contribution to the photoemission kink in the copper oxide superconductors. Nature 2008, 452(7190):975–978. 10.1038/nature06874
Acknowledgements
We thank Z.X. Shen and A. Fujimori for useful discussions and K. Ichiki, Y. Nakashima, and T. Fujita for their help with the experimental study. The ARPES experiments were performed under the approval of HRSC (Proposal No. 07A2, 09A11 and 10A24).
Author information
Affiliations
Corresponding author
Additional information
Competing interests
The authors declare that they have no competing interests.
Authors’ contributions
AI wrote the manuscript. HA and AI designed the experiment and analyzed the data with support from MT. HA acquired the ARPES data with support from AI, MA, and HN. Highquality singlecrystalline samples were grown by MI, KF, SI, and SU. All authors discussed the results and commented on the manuscript. All authors read and approved the final manuscript.
Authors’ original submitted files for images
Below are the links to the authors’ original submitted files for images.
Rights and permissions
Open Access This article is distributed under the terms of the Creative Commons Attribution 2.0 International License (https://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
About this article
Cite this article
Ino, A., Anzai, H., Arita, M. et al. Doping dependence of lowenergy quasiparticle excitations in superconducting Bi2212. Nanoscale Res Lett 8, 515 (2013). https://doi.org/10.1186/1556276X8515
Received:
Accepted:
Published:
DOI: https://doi.org/10.1186/1556276X8515
Keywords
 HighT_{c} cuprate
 Bi2212
 ARPES
 Superconducting gap
 Effective mass
 Coupling strength
 74.25.Jb
 74.72.h
 79.60.i